- 206 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about 'Mechanical Properties of Glass' - cedric

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

Mechanical Properties of Glass

- Elastic Modulus and Microhardness

[Chapter 8 – The “Good Book”*]

- Strength and Toughness [Chapter 18]
- Fracture mechanics tests
- Fractography
- Stress Corrosion
- Fracture Statistics

*A. Varshneya, “Fundamentals of Inorganic Glasses”,

Society of Glass Technology (2006)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Bond Breaking Leads to Characteristic Features

Log v

U

s

Kc

e

r

Log K = Log (Ys c ½)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Elastic Modulus Is Related To The Strength of Nearest Neighbor Bonds

F

U

r0

r

r0

r

Force = F = - dU/dr

Stiffness = S0 = (dU2/dr2) r = r0

Elastic Modulus = E = S / r0

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Elastic Modulus – Governs Deflection

S

e

Hardness Measures Surface Properties

Strength – Governs Load Bearing Capacity

Toughness – Governs Crack Propagation

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Stress = P / A

A = Cross-sectional Area = p r 2

P = Load On Sample

r

P

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Strain = DL / L

A = Cross-sectional Area = p r 2

L

L = Length

DL = Change In Length

DL

r

P

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Infinitesimal cube represents triaxial state of stress.

ey = (1 /E)[sy - n( sx+ sz)] gxy = [2(1+n) / E] (txy)

ex = (1 /E)[sx - n( sy+ sz)] gyz = [2(1+n) / E] (tyz)

ez = (1 /E)[sz - n( sy+ sx)] gzx = [2(1+n) / E] (tzx)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Special Cases of Loading Often Occur

(a) Tensile stress. (b) Shear stress. (c) Hydrostatic pressure.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

In uniaxial loading in the x direction, E (or Y) relates the stress, sx, to the strain, ex.

sx = E ex

- ey = ez= - n ex
- sxy = G g

p = K DV

s

e

Virtual Course on Glass - The Properties of Glass: Charge Conduction in Glass - Lecture 1

In the case of shear loading, the shear modulus is appropriate

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

(a) Tensile stress. (b) Shear stress. (c) Hydrostatic pressure.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

In the case of hydrostatic pressure, the bulk modulus is appropriate.

s

D V/ V0

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

There is a relationship between E, G and K (and of course Poisson’s ratio, n)

G = E / [2 (1+n)]

K = E / [3(1-2n)]

Note: -1 ≤ n ≤ 0.5.

(When n = 0.5, K ∞ and E 3G. Such a material is called incompressible.).

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

There is a relationship between E, G and K (and of course Poisson’s ratio, n)

G = E / [2 (1+n)]

K = E / [3(1-2n)]

So, when we determine any two parameters, (for isotropic materials) we can calculate the others.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

There are several techniques used to measure the elastic modulus:A. Stress-strain directly (load-displcament) 1. tension 2. 3-pt flexure 3. 4-pt flexure 4. Hydrostatic pressure 5. Torque on rodB. Ultrasonic wave velocity 1. Pulse echo 2. Direct waveC. Beam Vibration

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Elastic Modulus = Stress / Strain

P

A = Area = p r 2

S or s

A = Brittle

B = Ductile

Strain = e or e

S =Stress = P / A

r

Strain = DL / L

P

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

To measure E from flexure, need to calculate the stress and strain.

P

b

d

h

A

A

s = 3PL / (2 b h2) e = d / L

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Pulse echo technique is often used to measure modulus

C. Kittel, Intro. To Solid State Physics, J. Wiley & Sons

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Pulse Echo technique is one of the most reliable.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

In the simplest case for isotropic materials there are direct relationships.

vL = [ E / r]1/2

(Longitudinal waves)

vS = [ G / r]1/2

(Shear waves)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

For the beam vibration technique, we stimulate the flexural modes.

For beam bending:

E = (0.946 L4 f2r S) / h2

f = frequency

S = shape factor

H = width and height

L = length

r = density

Fig 8-5

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

In general, E decreases as the size and concentration of the alkali cations increases

Fig 8-6a

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

E decreases as the size and concentration of the alkali cations increase

E

K

n x 100

G

Fig 8-6b

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

E decreases as the size and concentration of the alkali cations increases

Fig 8-6c

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

E increases with addition of metal oxide (MO) [except PbO]

Na2O x MO 5SiO2

Fig.8-7 (Varshneya)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Lithia-aluminosilicates have greater E values than SiO2

Fig.8-8

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

In general, bulk moduli of silicate glasses increase with temperature (except at low temperatures [0 - 60K])

N.B. - the compressibility, k, is being graphed in the figure (Fig. 8-9).

(The compressibility is the reciprocal of the bulk modulus.)

Virtual Course on Glass - The Properties of Glass: Charge Conduction in Glass - Lecture 1

Composition and structure affect the values of elastic moduli.

N.B.: at low (< 10mol%) alkali content, E with B2O3 addition.

However, with greater alkali content glasses addition of B2O3 leads to a maximum in E.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Complications of silicate glasses makes predictions difficult

F = [-a / rn ]+ b / rm

(Condon-Morse)

Force = F = - dU/dr

Stiffness = S0 = (dU2/dr2) r = r0

Elastic Modulus = E = S / r0

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Complications of silicate glasses makes predictions difficult

F = [-a / rn ]+ b / rm

(Condon-Morse)

Force = F = - dU/dr

Stiffness = S0 = (dU2/dr2) r = r0

Elastic Modulus = E = S / r0

- General rules:
- E increases as r0x decreases
- E increases as valence, i.e., qa x qc
- E affected by bond type (covalent, ionic, metallic).
- E affected by structure (density, electron configuration, etc.)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Microhardness is a measure of surface properties and can be related to elastic modulus, toughness and surface tension.

Hardness = Force / Area

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Many hardness tests are available

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

The most common microhardness diamond tips for glasses are Vickers and Knoop

Fig. 8-12

Hardness = Force / Area

Hv = 1.854 F / D2 (Actual area) KHN = 14.23 F / L2 (Projected area)

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Note plastic flow in silicate glass using a Vickers microhardness indenter.

Plastic flow in Se glass using a Brinell microhardness indentation.

Fig. 8-13 a & b

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Diamond hardness indentations can result in elastic and plastic deformation.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Microhardness can be measured dynamically

HvL = 37.84 F / h2max

(from loaded depth, hmax)

Hvf = 37.84 F / h2f

(from unloaded depth, hf)

Refs. 34 and 35 in Chapter 8.

F = a1h + a2 h2 (equation fit to curve)

HvL2 (GPa)= 37.84 a2 { load independent hardness; a2 = N/mm2}

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Microhardness can be measured dynamically

Measure dF/dh on initial unloading

Er = (p / 2 A) [dF/dh]

Er =[(1-n2)/E] + [(1-ni2)/ Ei

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

- The energy spent during the nanoindentation process can be categorized as plastic energy (Wpl) and elastic energy (Wel). The indenter penetrates the sample and reaches the maximum penetration (hmax) at Pmax. During the unloading process, the compressed zone recovers and the final depth of the indent (hf)

is often much less than hmax.

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Elastic Moduli and microhardness are two important mechanical properties.

Elastic modulus is a macroscopic measure of the strength of bonds at the atomic scale.

Hooke’s law (stress proportional to strain) defines the moduli of linear elastic solids.

For isotropic glasses only two constants are required – others can be calculated. Note: -1 ≤ n ≤ 0.5. (When n = 0.5, K ∞ and E 3G).

Elastic modulus is best measured using the “pulse echo” or similar technique. For silicate glasses, E 70≈ GPa and n ≈ 0.22.

Hardness is a measure of the resistance to penetration. Both densification and material pile-up are observed in glasses.

Vickers indentation is the most common diamond indenter for glasses.

For a silicate glass, H v ≈ 5.5 GPa

Virtual Course on Glass - The Properties of Glass: Mechanical Properties of Glass - Lecture 11

Download Presentation

Connecting to Server..